pharmaceutical contaminants biodegradable nano carbon ... · pdf file biodegradable nano...
Click here to load reader
Post on 16-Mar-2020
Embed Size (px)
Biodegradable Nano Carbon based Smart Filters for Efficient Remediation of
Indu Tripathi,1,2 Laurel K. Dodgen,3 Fatemeh Ostadhossein,1,2 Santosh K. Misra,1,2 Enrique
Daza,1,2 Brajendra K. Sharma,3 Wei Zheng3 and Dipanjan Pan*1,2
1Departments of Bioengineering, Materials Science and Engineering, University of Illinois at
Urbana Champaign, Urbana, Illinois 61801, USA.
2Carle Foundation Hospital, Urbana, Illinois, 61801, USA.
3Illinois Sustainable Technology Center, Prairie Research Institute, University of Illinois at Urbana
Champaign, Champaign, Illinois, 61820, USA.
*Correspondence and requests for materials should be addressed to D.P. (email:
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A. This journal is © The Royal Society of Chemistry 2018
Figure S1. Size distribution of CNP-TCDA particles from TEM.
Figure S2. Thermal conversion of (a) TCDA to (b) polyTCDA.
Figure S3. Scavenging of various parent pharmaceutical moieties using PNCS. Scavenging of (a)
bis-phenyl amine; (b) anthracene and (c) mixture of polyaromatic hydrocarbons.
Figure S4. Representational dual mode interaction of PPCP (e.g. triclocarbon 3-(4-Chlorophenyl)-
1-(3,4-dichlorophenyl) urea) with PNCS.
Figure S5. Chemical structure of PPCPs and their scavenging % by PNCS.
Table S1. TOC (%) of PNCS treated samples compared to untreated PPCPs.
(%) TOC of PNCS treated samples compared to untreated Pharmaceutical compound name Round 1 Round 2 Round 3
Carbamazepine 23.0±2.3 27±2.7 -13±1.3
Gemfibrozil 13.0±1.3 6±0.6 -8±0.8
Triclocarbon -9.0±0.9 22±2.2 20±2.0
Table S2. Effect of filtration on % TOC.
(%) TOC of PNCS treated samples compared to untreated Pharmaceutical compound name Use 1 Reuse 1 Reuse 2
Carbamazepine 1±0.1 19±0.2 14±1.4
Gemfibrozil 4±0.4 13±1.3 8±0.8
Triclocarbon 1±0.1 8±0.8 11±1.1
Table S3. Reuse of PNCS and efficiency of pharmaceutical contaminant removal.
(%) Removal efficiency after PNCS
Pharmaceutical compound chemical
structure Use 1 Reuse 1 Reuse 2
Carbamazepine >99 11±1 5±0.5
Gemfibrozil >65 1±0.1 5±0.5
Triclocarbon >99 >99 >99
Materials and Methods
PPCP standards carbamazepine, gemfibrozil, and triclocarban were obtained from Restek
(Bellefonte, PA, USA). Isotopic standards including D10-carbamazepine, D6-gemfibrozil, and
13C6-triclocarban were purchased from Cambridge Isotope (Andover, MA, USA). Nectar agave
(HoneyTree’s Organic Agave Nectar, Onsted, MI) was procured from local grocery store, 10, 12-
tricosadiynoic acid from Sigma-Aldrich (St. Louis, MO). Poly(2-vinyl naphthalene-b-acrylic acid)
as the diblock copolymer was acquired from Alfa Aesar (Haverhill, MA). Solvents used in the
study, including methanol, acetone, and acetonitrile, were purchased from Fisher Scientific (Fair
Lawn, NJ, USA). Deionized (DI) water (>18.2 MΩ-cm) was supplied by a Labconco Water Pro
Plus system (Kansas City, MO, USA).
Preparation of Pharmaceutical-Nano-Carbo-Scroungers (PNCS) .
The absorption-based remediation of pharmaceutical contaminants requires a multi-component
nano-architecture which can create a hydrophobic inner compartment for entrapment. Our strategy
utilizes a biodegradable carbon core hydrophobically modified by a cross linker, 10,12-
tricosadiynoic acid (TCDA). It could be produced by thermally cross-linking TCDA onto
commercially available agave nectar (an inexpensive sweetener composed of 47-56% of fructose
and 19-20% glucose).
The CNP-TCDA core of the PNCS was produced by a hydrothermal method1-5 of
controlled heating in a suspension of 1250 mg/ml of nectar agave (HoneyTree’s Organic Agave
Nectar, Onsted, MI) and 187.5mg/ml of 10, 12-tricosadiynoic acid (Sigma-Aldrich, St. Louis, MO)
in nanopure water in a 20 ml scintillation vial at 250 degrees Celsius for 45 minutes or until all
water evaporates and product turns black mass. It was allowed to be soaked in THF overnight then
resuspended by sonication (Q700, Qsonica Sonicators, Newtown, CT) in an ice bath (to prevent
evaporation) for 24 minutes at one amplitude with intervals of five seconds on and three seconds
off. The sonicated suspension was filtered through 0.45μm and 0.22μm PTFE membranes
sequentially. Prepared suspensions were characterized for physiochemical characteristics and
found to be of Nano dimensions. The suspension was dried out to produce a residue. This residue
and Poly (2-vinyl naphthalene-b-acrylic acid) as our diblock copolymer. t a 10:2 mass ratio
respectively, was resuspended in THF. The volume of THF used is the minimum required to fully
dissolve solutes. The crosslinking was monitored using a UV-VIS Spectroscopy (GENESYS 10
S). To measure the collected samples, a 1 to 20 dilution of the heated sample was prepared in
deionized water for each UV-VIS measurement where a stock solution of agave in water at the
same concentration was used as a blank. Water was then added rapidly to THF suspension of
particle mass at a twice the volume of THF to produce the block polymer coated nanoparticles
known as the pharmaceutical Nanocarboscavenger (PNCS). This suspension was placed in a
vacuum to dry and then scraped and ground into powder form.
Dynamic Light Scattering
The hydrodynamic size distribution of the CNP-TCDA was determined through dynamic light
scattering measurements on a Malvern Zetasizer ZS90 instrument (Malvern Instruments Ltd,
United Kingdom) at fixed angle of 90. A 10 μL of particle suspension was mixed with 990 μL of
THF to run the samples in DLS machine. A photomultiplier aperture of 400 nm was used, and the
incident laser power was so adjusted to obtain a photon counting rate between 200 and 300 kcps.
Measurements for which the measured and calculated baselines of the intensity autocorrelation
function were within 0.1% range were used for diameter values. All measurements were carried
out in triplet of thirteen consecutive measurements. Similarly, hydrodynamic diameter of PNCS
was determined in water medium.
UV-Vis Spectroscopic Study
The absorbance of the PNCS suspensions (0.1 mg/mL) and aromatic hydrocarbons dissolved in
water were recorded in spectrum range of 200 to 800 nm on a GENESYS 10 UV−Vis
spectrophotometer (Thermo Scientific).
Transmission Electron Microscopy (TEM)
Anhydrous state morphology and size of PNCS were acquired by transmission electron
microscopy. A 5 μL volume of 0.1 mg/mL PNCS was coated on copper grid and air dried before
being dried under vacuum for 4h. TEM was acquired on JEOL 2100 Cryo TEM at MRL, UIUC
PCCP Scavenging Procedure
Briefly, three PPCP stock solutions (Carbamazepine, gemfibrozil and triclocarban) were added to
deionized water and mixed thoroughly, yielding initial concentration of 0.2 µg/L. Five milliliters
of each samples were taken in 20 ml scintillation vial and 10 mgs of PNCS added to it. Magnetic
stir bars were put in the scintillation vial and stirred for 24hrs. This treatment was repeated three
times. The treated samples centrifuged at 11,000 rpm for 10 minutes and then filtered through a
0.45-µm membrane (Iso-Disc, Supelco, Bellefonte, PA) using a syringe. All samples were stored
at 4oC and analyzed within a week using liquid chromatography tandem-mass spectrometry (LC-
MS/MS). Preliminary experiments showed that targeted PPCP concentrations were stable at this
temperature and time period.
Concentrations of PPCPs were determined by LC-MS/MS (Waters, Quattro Macro, QA1140,
Milford, MA) based on our previously developed methods (Li et al., 2013). Isotopic standard (100
ng for each chemical) was spiked into the sample extract and 30 μL of sample was injected for
analysis. Three PPCPs investigated in this work were separated on a symmetry C18 column (3.5
µm particle size, 2.1×150 mm, Waters) by a high-performance liquid chromatography (HPLC)
system (2695 module, Waters). A gradient separation was achieved using two mobile phases:
solvent A, water containing 0.1% ammonium acetate and 0.1% acetic acid; and solvent B, 1:1
methanol: acetonitrile. The gradient started with 90% solvent A and 10% solvent B and was
maintained for 2 minutes. Then the gradient was ramped up to 5% solvent A and 95% solvent B
linearly in 13 minutes and maintained for 8 minutes. The gradient was changed back to 90%
solvent A and 10% solvent B after 0.5 minutes and re-equilibrated for 5.5 minutes. The flow rate
was 0.19 mL/min.
The HPLC system was coupled with a Quattro Macro mass spectrometer (QA1140,
Waters, Milford, MA) equipped with an electrospray ionization (ESI) source. For the measurement
of three targeted PPCPs, the mass spectrometer was operated in positive and nega